820 Biomacromolecules 2010, 11, 820–826
Cytocompatibility and Uptake of Halloysite Clay Nanotubes
Viviana Vergaro,† Elshad Abdullayev,‡ Yuri M. Lvov,‡ Andre Zeitoun,§ Roberto Cingolani,†
Ross Rinaldi,† and Stefano Leporatti*,†
National Nanotechnology Laboratory (NNL) of CNR-INFM, Italian Institute of Technology (IIT) Lecce Unit,
University of Salento, ISUFI Lecce, 73100 Italy, Institute for Micromanufacturing and Biomedical
Engineering Program, Louisiana Tech University, 911 Hergot Avenue, Ruston, Louisiana 71272, and
Applied Minerals, Inc., New York, New York
Received December 19, 2009; Revised Manuscript Received January 29, 2010
Halloysite is aluminosilicate clay with hollow tubular structure of 50 nm external diameter and 15 nm diameter
lumen. Halloysite biocompatibility study is important for its potential applications in polymer composites, bone
implants, controlled drug delivery, and for protective coating (e.g., anticorrosion or antimolding). Halloysite
nanotubes were added to different cell cultures for toxicity tests. Its ﬂuorescence functionalization by
aminopropyltriethosilane (APTES) and with ﬂuorescently labeled polyelectrolyte layers allowed following halloysite
uptake by the cells with confocal laser scanning microscopy (CLSM). Quantitative Trypan blue and MTT
measurements performed with two neoplastic cell lines model systems as a function of the nanotubes concentration
and incubation time indicate that halloysite exhibits a high level of biocompatibility and very low cytotoxicity,
rendering it a good candidate for household materials and medicine. A combination of transmission electron
microscopy (TEM), scanning electron microscopy (SEM), and scanning force microscopy (SFM) imaging techniques
have been employed to elucidate the structure of halloysite nanotubes.
Introduction the main prerequisites for safe usage of halloysite in the delivery
of biologically active substances in medical and household
Halloysite clay is a two-layered aluminosilicate, chemically products.
similar to kaolin, which has hollow tubular structure in the However, a comprehensive study of halloysite biocompat-
submicrometer range.1-3 Kaolin sheets are rolled into tubes ibility has not been done yet. Are there health risks associated
because of the strain caused by lattice mismatch between with halloysite? Currently, there is no research on cytotoxicity
adjacent silicone dioxide and aluminum oxide layers.1,2 As for caused by cellular exposure to halloysite in concentrations viable
most natural materials, the size of halloysite particles varies from for commercial applications. HNTs are rolled versions of kaolin,
50 to 70 nm in external diameter, ca. 15 nm diameter lumen and they are just as chemically stable as widely used in
and 1 ( 0.5 µm length. Halloysite nanotubes (HNTs) are capable household products kaolin clay. However, concern over the use
of entrapping a range of active agents within the inner lumen, of ﬁne particles rich in silica is understandable. Many diseases,
followed by their retention and slow release.3-13 such as ﬁbrosing collagenous pneumoconiosis and silicosis, are
related to prolonged lung exposure to ﬁne crystalline silica
There is an increasing amount of research ongoing to produce particles. Studies associate pathogenesis of these diseases to (1)
functional nanometer-scale containers, and there is growing generation of free radicals by the particles and (2) overactive
demand for their use in biomedical applications. Such containers inﬂammatory response by intra-alveolar/interstitial macrophages.
would be inexpensive materials with a simple means of In this article, we focused on studying HNTs interaction (both
fabrication, and thus natural resources and nanotubes are good untreated and ﬂuorescently labeled) with cells. We analyzed
candidates for this. Different chemistry of the inner and outer halloysite toxicity and visualized the process of cell uptake of
surfaces in halloysite tubes would also allow for separate ﬂuorescently labeled clay nanotubes with confocal laser scanning
modiﬁcation of inner and outer walls, for example, for selective microscopy (CLSM). Intracellular uptake by cells of different
labeling. The lumen diameter of halloysite tube ﬁts well to origins (cervical adenocarcinoma, HeLa, or breast cancer cells,
macromolecule and protein diameters, allowing their encasing MCF-7) and cytoviability tests (MTT and Trypan blue) dem-
in the tube. Halloysite is a natural product which will not add onstrated halloysite cytocompatibility and potential as biof-
risk to the environment. riendly cargo nanocontainer for biomaterials.
Halloysite was found to be a viable and inexpensive nanoscale
container for encapsulation of drugs that was ﬁrst demonstrated Materials and Methods
by Price, Lvov, and Kelly, et al.3-5 Polymer-halloysite com-
Chemicals. The sources of the chemicals are as follows: poly
posites are perspective materials for medical implants, for (sodium 4-styrene-sulfonate) (PSS, Sigma), poly (allylamine hydro-
example, for bone repairing.5,14–16 Biocompatibility is one of chloride) (PAH, Sigma), fetal bovine serum (FBS, Sigma), penicillin-
streptomycin solution (Sigma), sodium pyruvate (Sigma), DMEM
* To whom correspondence should be addressed. E-mail: stefano.leporatti@ medium (Sigma), thiazolyl blue tetrazolium bromide >97.5% TLC
University of Salento.
(Sigma), phosphate-buffered saline, Dulbecco A (PBS, Oxoid), sepha-
Louisiana Tech University. dex G25 (Sigma), ﬂuorescein isothiocyanate isomer I (FITC, Aldrich),
Applied Minerals, Inc. triton X-100 (Sigma), aminopropyltriethoxysilane (APTES, 99%,
10.1021/bm9014446 2010 American Chemical Society
Published on Web 02/19/2010
Halloysite Nanonotube Cytocompatibility and Uptake Biomacromolecules, Vol. 11, No. 3, 2010 821
Aldrich). Puriﬁed dehydrated HNTs were obtained from Applied Scanning Force Microscopy (SFM). SFM micrographs were
Minerals, Inc. obtained with Bioscope II and Multimode-Picoforce (Veeco Instruments
Halloysite Labeling. Halloysite Fluorescence Staining by Amino- Inc.) in air at room temperature using contact mode with MLCT-AUNM
propyltriethoxysilane Functionalization. We labeled HNTs by modify- cantilevers of 0.01 N/m spring constant and in tapping mode using
ing their surface with aminopropyltriethoxysilane (APTES). Modiﬁed TESPA cantilevers of 4N/m spring constant. A drop of sample
halloysite samples were prepared according to the procedure generally suspension was applied to a freshly cleaved mica support. HNTs were
applied for the grafting of silica-based materials.15 APTES (500 µL) imaged after their dehydration. Images were analyzed by Nanoscope
was dissolved in 6.25 mL of toluene; 0.15 g of clay powder was added, software (version 7.30s1rs2) and by SXM image (v.188, by Steve
and the suspension was dispersed ultrasonically for 30 min. The Barrett, England) (Figure 3A). Figure 3C has been processed by WSXM
suspension was then reﬂuxed at 120 °C for 20 h under constant stirring. (20).
The resultant mixture was extensively washed with fresh toluene six Confocal Laser Scanning Fluorescence Microscopy. Confocal
times to remove the excess organosilane and then dried overnight at micrographs were taken with a confocal scanning system Leica TCS
120 °C for further curing. The mixture was then washed 10 times with SP5 (Leica Microsystem GmbH, Mannheim, Germany) and equipped
DI water, and the sample was freeze-dried overnight. The amino with a 63× oil immersion objective. Z scan and XY scans images were
functionalized nanotubes (HNTs, 3 mg) were dispersed in 1.5 mL of acquired to demonstrate internalization of nanotubes into cells.
0.1 M carbonate buffer (pH 8.0). To this solution 100 µL of 13 mM Cytotoxicity Analysis. MTT Assay. All cell lines described above
solution of FITC in DMSO was added. The mixture was allowed to were used in the general cytotoxicity test. The MTT system is measuring
react for 2 days under constant stirring at room temperature and the activity of living cells via mitochondrial dehydrogenase activity.
protection from light. The solution was dialyzed and lyophilized The halloysite suspensions at different concentration (from 1 µg/mL
overnight. to 1 mg/mL) were diluted with complete culture medium. The MTT
Layer-by-Layer Coating. HNTs were coated using a layer-by-layer method of cell determination is most effective when cultures are
(LbL) technique via alternate adsorption of polycations and polyanion.17–19 prepared in multiwell plates. HeLa and MCF-7 cells (105 cells/mL)
HNTs are negatively charged in water with a ζ potential of -40 mV were added to six-well culture plates at 2 mL/well and incubated with
at pH 6.5. Halloysite dispersed in DI water (1 mL) was mixed with a the nanotubes at 37 °C in 5% CO2, 95% relative humidity for 24 to 48
solution containing 2 mg/mL of positively charged poly(allylamine to 72 h. The control was a complete culture medium. After an
hydrochloride) (PAH). The dispersion was continuously shaken for 10 appropriate incubation period, cultures were removed from the incuba-
min. The excess polycation was removed by three centrifugation/ tor, and an MTT solution in the amount equal to 10% of the culture
volume was aseptically added. Cultures were returned to incubator and
washing steps with DI water. Thereafter, 1 mL of a 0.5 M NaCl solution
incubated for 3 h. After the incubation period, cultures were removed
containing 3 mg/mL of negatively charged poly(sodium 4-styrene-
from the incubator, and resulting MTT formazane crystals were
sulfonate) (PSS) was added, and the dispersion was continuously shaken
dissolved with acidiﬁed isopropanol solution at equal volume with
for 10 min, followed by three centrifugation/washing steps. This
culture. The plates were ready within 1 h after acidiﬁed isopropanol
procedure was repeated three times, resulting in the deposition of ﬁve
solution was added. After the incubation time, pipetting up and down
polyelectrolyte layers. FITC-labeled PAH layer was inserted into the
was required to dissolve completely the MTT formazane crystals. An
multilayer to follow HNTs uptake by cells. To prepare PAH-FITC,
absorbance at wavelength of 570 nm was measured with Agilent 4853
two solutions (PAH and FITC) were mixed at a ratio of 1:5 (PAH/
UV-vis spectrophotometer. Subtract background absorbance was
FITC), incubated over 2 to 3 days, and then dialyzed against water for
measured at 690 nm. The viability percentage was expressed as the
1 to 2 h, followed by drying in lyophilizator and dissolving in water.
relative growth rate (RGR) by equation
Finally, free FITC was removed with a Sephadex G25 column in
ammoniac buffer (pH 8.5), dried within lyophilizator, and stored at
+4 °C before being used in LbL assembly. The ﬁnal architecture of RGR ) (Dsample/Dcontrol)100%
the ﬂuorescent LbL coating for halloysite was PAH/PSS/PAH-FITC/
where Dsample and Dcontrol are the absorbances of the sample and the
Cell Culture. Human epithelial adenocarcinoma cell line (HeLa)
and human breast cancer cell line (MCF-7) were maintained in DMEM
Trypan Blue Assay. Trypan Blue is one of the dye exclusion
medium supplemented with FBS (10%), penicillin (100 U/mL culture
procedures for viable cell counting. This method is based on the
medium), streptomycin (100 µg/mL culture medium), glutamine (5%),
principle that live (viable) cells do not take up certain dyes, whereas
and sodium pyruvate (5%). Cells were grown in a humidiﬁed incubator
dead (nonviable) cells do. Live cells with intact cell membranes are
at 37 °C, 5% CO2, and 95% relative humidity.
not colored. Because cells are very selective in the compounds that
Halloysite ξ-Potential Characterization. Halloysite surface poten-
pass through the membrane, in a viable cell, Trypan blue is not
tial was analyzed by using microelectrophoresis (ZetaPlus Potential
absorbed; however, it traverses the membrane in a dead cell. Therefore,
Analyzer, Brookhaven Instruments). For this purpose, diluted aqueous dead cells are shown to be a distinctive blue color under a microscope,
dispersion of halloysite (ca. 1 µg/mL) was transferred into the special and living cells are excluded from staining. For the trypan blue assay,
cuvette, and electric ﬁeld was applied across the suspension, causing HeLa and MCF-7 cells (105 cells/mL) were added to six-well culture
the movement of negatively charged halloysite nanoparticles toward plates at 2 mL/well and incubated at 37 °C in 5% CO2, 95% relative
cathode. Surface electrical potential of the particles was determined humidity for 24 to 48 to 72 h with the nanotubes suspension. The
by Smoluchowski formula using particle speed measured with dynamic halloysite suspension at different concentration (from 1 µg/mL to 1
light scattering (all included in the instrument software). To change mg/mL) was diluted with complete culture medium, which is used as
the pH of the solution, HCl or NaOH were added to the suspensions. control. After the appropriate incubation period, the medium of each
A similar procedure was applied for silica and alumina colloids. well was collected. After trypsinization, the cells were collected and
Microscopy Imaging. Transmission Electron Microscopy (TEM). centrifuged. The pellet was resuspended in an appropriate amount of
TEM images were recorded with a Jeol Jem 1011 microscope operated medium. The collected cells were mixed with the same volume of 0.4%
at an accelerating voltage of 100 kV. We prepared samples for analysis trypan blue solution. Cells were allowed to stand from 5 to 15 min.
by dropping a dilute nanotube dispersion in water onto carbon-coated Later, 10 µL of stained cells was placed in a hemocytometer, and the
copper grids and then allowing water to evaporate. number of viable (unstained) and dead (stained) cells was counted with
Scanning Electron Microscopy (SEM). Nanotube external surface a light microscope. The viability percentage was expressed using the
morphology was characterized by a scanning electron microscope type following equation: cell viability (%) ) total viable cells (unstained)/
Hitachi S 4800 FE-SEM; the tube samples were coated with 1 nm Pt. total cells (stained and unstained) × 100.
822 Biomacromolecules, Vol. 11, No. 3, 2010 Vergaro et al.
Figure 1. Comparison of ξ-potential curves for halloysite nanotubes
(violet), silica (blue), and alumina (red) nanoparticles.
Figure 2. (a) SEM image of halloysite nanotubes powder, as supplied
Nanotubes Uptake by Cells. QualitatiVe Study. To determine the
from Dragon Mine, Applied Minerals, Inc. TEM images of halloysite
cellular uptake of the nanotubes, we seeded 105 cells/mL in sterile glass- clay nanotubes: (b,c) longitude and (d) cross-section.
culture slide coated with poly-L-lysine. The cells were incubated with
the coated-nanotube dispersions. After 3 h of incubation at 37 °C, the
culture medium was removed, and cells were washed three times with of external loosely packed aluminosilicate layers that are not
phosphate-buffered saline and ﬁxed in formaldeyde 3.7%. After that, well resolved in TEM image because they are only 1 to 2 nm
cells were stained with phalloidin and hoechst and processed by thick but may be detected with SFM. An additional argument
confocal microscopy. for this could be the very small value of elasticity modulus
measured (ca. 200 kPa). HNT elasticity is considerably smaller
than that of carbon nanotubes (CNTs), which usually have a
Results Young’s modulus of ∼1 TPa.20,21 Such large differences in
Characterization of Halloysite Nanotubes. HNTs form elastic properties between CNTs and HNTs could facilitate HNT
stable colloids in water in wide pH range. Figure 1 shows that internalization into cellular compartments, enhancing spontane-
halloysite is negatively charged above pH 2.4 with ζ-potential ous penetration.
reaching -50 mV at pH 6 and higher. High ζ-potential is a Imaging Halloysite Nanotubes Uptaken by the Cells. To
condition of good colloidal stability of dispersed nanotubes. An study halloysite cytotoxicity, we added these clay nanotubes
interesting feature is that because of different outside and inside (both ﬂuorescently labeled and unlabeled) to two model cell
chemistry (which comprise silica, SiO2, and alumina, Al2O3, cultures (MCF-7 (breast cancer) and HeLa (cervical cancer)
sheets, correspondingly) the tube lumen is charged positively, cells). Figures 4 and 5 demonstrate halloysite uptake by cells.
whereas the external surface is charged negatively. This property In Figure 4, two orthogonal XZ sections of a Z-stack for MCF-7
of the tubes allows loading of negative molecules selectively and HeLa are shown. In the bottom and right sides of the Figure
into the lumen at the range of pH from 2.5 to 8.5. In the same 4A, the MCF-7 cell cytoskeleton (red, TRITC-labeled) with
Figure 1, for comparison, we present the ζ-potential of silica colocalized HNTs of yellow color, merging from FITC-labeled
and alumina demonstrating this “window” of oppositely charged HNTs (green) and phalloidin-TRITC-labeled cytoskeleton (red)
internal and external surfaces. are shown. Similarly, in the bottom and right sides of the Figure
Figure 2 shows electron microscopy images, SEM (a) and 4B the localization of HNTs (green) outside HeLa nuclei (blue,
TEM (b-d), obtained from halloysite spread on ﬂat support Hoechst staining) is illustrated. HNTs accumulate all over the
(a,c) and obtained from halloysite embedded into PMMA (b,d). cell colonies (yellow coverage over red cytoskeleton). These
One can see that the majority of the sample consists of images demonstrate effective internalization of HNTs in the
cylindrical tubes of 40-50 nm diameter and length of 0.5 to 2 cells.
µm. HNTs are rather polydisperse in length. TEM images clearly In Figure 5, we report confocal micrographs of MCF-7 (a-c)
indicate the empty lumen of the halloysite with 15-20 nm and HeLa (d-f) cells interacting with HNTs (ﬂuorescent-labeled
diameters. For some tubes, one can see loose packing of the either by LBL or by APTES) showing colocalization of HNTs
outermost alumosilicate sheets, which are not tightly rolled aggregates (green) around cell nuclei (blue). One can see that
(Figure 2c). in both cases, labeled halloysite readily penetrates the cells
SFM images (Figure 3) reveal the surface morphology of the (green area around blue cell nuclei). LbL-coated HNTs contain-
tubes demonstrating the rolled nature of the tubes. SFM ing FITC-labeled layer (green) were analyzed for breast cancer
micrographs are acquired both in tapping mode (Figure 3a) and cells, MCF-7. APTES-FITC-processed halloysite gives brighter
in contact mode (Figure 3b). Figure 3b shows a deﬂection (error images, indicating better FITC labeling. LbL polyelectrolyte
signal mode) contact mode SFM image of two isolated tubes, multilayer coating had lower image sensitivity as compared with
enhancing morphological details. Halloysite particles appeared tube labeling through APTES-FITC. HNTs are readily uptaken
to be rolled cylindrically, as shown in the 3D view of a long by cells, predominantly in the cytoplasmatic region (outside
isolated tube. The tube diameter measured from SFM is ca. 100 nuclear regions, blue). A similar result was obtained for APTES-
nm (see inset in Figure 3b), which is larger than the one functionalized HNTs (green), but HeLa cells were used in this
measured from TEM images. It may be related to SFM tip size case instead of MCF-7 (Figure 5e,f).
(which has a radius of curvature of around 20 nm) convolution. Halloysite Cytotoxicity. Uncoated Halloysite. Figures 6 and
Another reason for larger SFM diameter may be the presence 8 summarize data on cytotoxicity of halloysite studied with
Halloysite Nanonotube Cytocompatibility and Uptake Biomacromolecules, Vol. 11, No. 3, 2010 823
Figure 3. (a) Tapping mode SFM image of halloysite clay nanotubes (Z scale 700 nm). (b) Contact mode (deﬂection) image of two isolated
nanotubes. A typical height proﬁle of a single nanotube is shown in the inset. (c) 3D view of a single long nanotube.
Figure 4. (a) CLSM image of halloysite nanotubes (HNTs) intracellular uptake by MCF-7 cells. Sections of a Z-stack FITC ﬂuorescence (green)
and phallloidin-TRITC ﬂuorescence overlaid images (image size: 108 mm). (b) CLSM image of HNTs (functionalized by APTES) intracellular
uptake by HeLa cells. Sections of a Z-stack FITC ﬂuorescence of HNTs+APTES (green) and Hoechst-ﬂuorescence-stained HeLa nuclei (blue)
overlaid images (image size: 42 mm).
human cell models: breast cancer cell line (MCF-7) and cervical the toxicity of APTES-FITC-functionalized HNTs for two cell
cancer cell (HeLa). We performed MTT tests at different time lines. HeLa and MCF-7 cell mortality increases with increasing
intervals (24 to 48 to 72 h) and at different concentrations (from concentration for both cells in a similar manner with uncoated
1 µg/mL to 1 mg/mL). The powder of halloysite was dispersed nanotubes.
in DI water and added to the cell cultures. In both cell lines,
the HNTs exhibited growth inhibition in a concentration- Therefore, uncoated and APTES-functionalized HNTs did not
dependent manner. The cell viability was preserved (ca. 70% the effect cell viability, and the trends in the cell viability were
of cells survived) up to halloysite concentration of 75 µg/mL the same. These toxicity data were also conﬁrmed by Trypan
(Figure 6 and 8). With increasing tube concentration up to 1000 blue tests performed under the same conditions as those for
µg/mL, there is a clear decrease in cell vitality (less pronounced nonfunctionalized nanotubes (Figure 8). These data show that
for longer incubation time). For MCF-7 cells, mortality was nanotubes were uptaken by cells, and their viability is main-
increasing for the same concentration range as for Hela cells. tained at >70% for HNT concentrations up to 75 µg/mL,
FITC-Labeled Halloysite. To follow halloysite localization suggesting high biocompatibility of halloysite. With increasing
into the cells and to study its uptake, we used nanotubes halloysite concentration, there is a signiﬁcant vitality reduction
functionalized with FITC, as described above. Figure 7 gives (Figure 8A,B).
824 Biomacromolecules, Vol. 11, No. 3, 2010 Vergaro et al.
Figure 5. CLSM images of halloysite nanotubes (HNTs) intracellular uptake by cancer cells. (a-c) CLSM images of HNT (coated by polyelectrolyte
multilayers with a FITC-labeled layer embedded herein) spontaneous intracellular uptake by MCF-7 cells. (a) Hoechst ﬂuorescence of nuclei
(blue). (b) FITC ﬂuorescence (green) of HNTs coated with an FITC layer embedded in polyelectrolyte multilayers. (c) FITC ﬂuorescence of
HNTs with a FITC layer and MCF-7 nuclei (blue) overlaid images. (d,e) CLSM images of HNT (functionalized by APTES) spontaneous intracellular
uptake by HeLa cells. (d) Hoechst ﬂuorescence of nuclei (blue). (e) FITC ﬂuorescence (green) of HNTs+APTES. (f) FITC ﬂuorescence of
HNTs+APTES and HeLa nuclei (blue) overlaid images.
Figure 6. MTT assay of halloysite taken up by (a) HeLa and (b)
MCF-7 cell percent cell viability versus halloysite concentration for
24 to 48 to 72 h (Error bar is STD (standard deviation), not visible).
Figure 7. MTT assay of halloysite nanotubes (HNTs) functionalized
with APTES on (a) HeLa (cervical cancer) and (b) MCF-7 cells.
Percent cell viability versus HNTs+APTES concentration for 24 to
48 to 72 h. (Error bar is STD (standard deviation), not visible).
Biocompatibility experiments were previously performed on Similarly, halloysite may be highly hydrated under biological
halloysite multilayer assembled on plastic or glass surface via conditions, which may result in high-level biocompatibility.
LbL process via alternated adsorption with cationic poly(eth- Very thin halloysite multilayer (ca. 300 nm) improved adhesion
yleneimine) or poly(lysine).10 Hydrogel formation through of human dermal ﬁbroblasts, and ﬁbroblasts maintained their
interaction between clay and polyelectrolytes was also re- cellular phenoptype on this coating. Fibroblast cell attachment
ported.11 This implies that claylike materials may have high and spreading was faster on halloysite-coated substrate as
afﬁnity to water in the presence of counter-charged materials. compared with silica and montmorillonite clay coating or bare
Halloysite Nanonotube Cytocompatibility and Uptake Biomacromolecules, Vol. 11, No. 3, 2010 825
nuclea. Of course, testing with other cells as well as small
animals will proceed to be driven by these clay nanotube
Studying halloysite toxicity, we had in mind blick data on
asbestos toxicity and its danger for living organisms.21,22 The
main difference of halloysite, as compared with asbestos
microﬁbers, is that these nanotubes are much shorter and thinner
and ﬁt the size window (0.5-1.5 µm), which is generally
considered to be not toxic for silicate nanoparticles.24 Halloysite
is just a rolled version of widely-adopted-in-human-life kaolin
clay (alumosilicate) and is chemically different from asbestos,
which is magnesium silicate (chrysolite), or less common Na
and Fe, Mg silicates (amphiboles). The danger of asbestos is
based on its very long ﬁber structure (5-20 µm length). In the
review on mechanisms of asbestos pathogenesis,23 it is indicated
that asbestos ﬁbers shorter than 5 µm are safer. Long thin ﬁbers
are more potent inducers of cell injury and inﬂammation.
Halloysite tube length of ca. 1 µm allows their easier removal
Another point is the concentration range: in our experiments,
halloysite concentration up to 75 µg /mL (ca. 1011 particles per
gram of cells) was safe for the cells, whereas asbestos disease
is caused by a much smaller number of asbestos ﬁbers per gram
of lung (ca. 108 particle per gram). Therefore, already 1000 times
less particle concentration of asbestos as compared with
halloysite causes a disease.
Generally speaking, cytotoxicity of asbestos ﬁbers is much
higher as compared with that of other minerals. Hart and
Figure 8. Trypan Blue test of halloysite nanotubes in (a) MCF-7 and
Hesterberg23 carried out studies showing moderate cytotoxic
(b) HeLa Cells. Percent cell viability versus halloysite concentration
for 24 to 48 to 72 h. effect of different silica-rich minerals as compared with asbestos.
There is a little inconsistency with different literature sources
as to what the threshold is for silica particle size for cytotoxic
glass.10 Later, similar results endorisng osteoblast and ﬁbroblasts or ﬁbrogenic effects, but in all publications, particles larger than
cell proliferation were obtained for composites of poly(vynil 5 µm were found to be more ﬁbrogenic than particles of 1 µm
alcohol) containing up to 5 wt % of halloysite.14 In all of these in diameter or less.22-24 Toxicity of halloysite may be compared
tests, biological cells were seeded on halloysite-containing with that of silica nanoparticles because its external surface
surfaces, and no data on HNTs penetration into cells were exposed to intracellular media is silica. Our results have shown
provided. that even large amounts of added halloysite (up to 75 µg/mL)
More halloysite exposure to biological tissue is expected if did not show toxicity, and at least 90% of the cells survived,
one applies HNTs for drug delivery or medical implants (such whereas from the ﬂuorescence laser confocal images, one could
as tooth ﬁllers or bone cements).3-5,9,10 For example, in the see that nanotubes were taken up by the cells. From our point
case of bone implants with typical size of ca. 1 cm2 of of view, direct toxicity of halloysite to cells will not be the
polymetmethacrylate-based cement loaded with 3 wt % of issue in applications, oppositely, for example, to CNTs, which
halloysite, it contains ca. 1010 clay nanotubes in the 10 µm kill cells.25,26 Polyelectrolyte nanotubes assembled in alumina
surface layer. Eventually, during a months-long degradation cylindrical pores could be another reference for our work.27
process, these clay nanoparticles may be released to connected These tubes have dimensions close to those of the HNTs and
biological tissue having mass of a few grams. Still, this also have low toxicity and were readily internalized into cancer
concentration of ca. 1 µg/mL is at least 100 times less than cells.
given above data on safe halloysite concentration. In ref 8, we
Secondary effects of HNTs on tissue may be essential, such
tested the toxicity of halloysite for 24 to 48 h of incubation
as increased ﬁbrogenicity, but it is not always harmful and may
time for ﬁbroblasts and human breast cells. It was observed
be even useful, for example, for bone implants. As the collective
that halloysite is nontoxic to these cells and is even much less
research stands, experimentation with macrophage exposure to
harmful than usual salt (NaCl). The percentage of live cells, as
halloysite seems appropriate and ultimately inevitable at the next
determined by celltiter-96 reagent, was measured for various
concentrations of testing agents (raw halloysite was added to
0.1 to 100 µg/mL of culture, and sodium chloride was a negative
Our data show that the addition of even as much as 75
µg /mL of halloysite in cell culture did not kill tested cells. With TEM, SEM, and SFM microscopy, we characterized
(For comparison, the addition of only 50 µg /mL of usual NaCl halloysite clay as tubular nanoparticles of ca. 50 nm external
killed all the cells.) Fluorescence confocal microscopy data diameter, 15 nm lumen diameter, and of 500-1500 nm length.
revealed that the cells accumulate halloysite in their interior, In wide range of pH, it has negative electrical ζ-potential of
but this does not prevent their proliferation. We were able to ca. -50 mV, which allows halloysite good dispersibility and
visualize the process of cellular uptake and have shown that colloidal stability in water. An addition of halloysite to two
HNTs penetrate into the cells and concentrate around the cell different cell lines demonstrated that it is nontoxic up to
826 Biomacromolecules, Vol. 11, No. 3, 2010 Vergaro et al.
concentrations of 75 µg/mL, whereas parallel laser confocal (12) Viseras, M. T.; Aguzzi, C.; Cerezo, P.; Cultrone, G.; Viseras, C.
visualization of cell uptake of ﬂuorescently labeled halloysite Supramolecular Structure of 5-Aminosalycilic Acid/Halloysite Com-
posites. J. Microencapsulation 2009, 26, 279–286.
demonstrated its location within the cells in the nuclear vicinity.
(13) Liu, M.; Guo, B.; Zou, Q.; Du, M.; Jia, D. Interaction between
The current research suggests that HNTs are not toxic for cells. Halloysite Nanotubes and 2,5-Bis(2-benzoxazolyl) Thiophene and
Their Effect on Reinforcement of Polypropylene Nanocomposites.
Acknowledgment. Financial support of Italian Ministry of Nanotechnology 2008, 19, 205709.
University and Research (MIUR) through FIRB project no. (14) Zhou, W.; Guo, B.; Liu, M.; Liao, R.; Rabie, A.; Jia, D. Poly(vinyl
RBLA03ER38 is gratefully acknowledged. “ Con il contributo alcohol)/Halloysite Nanotubes Bionanocomposite Films. J. Biomed.
del Ministero degli Affari Esteri, Direzione Generale per la Mater. Res., Part A 2009, 2, 1456–1463.
promozione e la Cooperazione Sociale ” (ItalysUSA Bilateral (15) Yuan, P.; Southon, P.; Liu, Z.; Green, M.; Hook, J.; Antill, S.; Kepert,
C. Functionalization of Halloysite Clay Nanotubes by Grafting with
Project “Nano-Carriers for Cancer Therapy”). We acknowledge Aminopropyltriethosilane. J. Phys. Chem. C 2008, 112, 15742–15751.
Applied Minerals, Inc. for providing halloysite and David Mills (16) Liu, P.; Zhao, M. Silver Nanoparticle Supported on Halloysite
(Louisiana Tech University) for data concerning halloysite bone Nanotubes Catalyzed Reduction of 4-Nitrophenol. Appl. Surf. Sci.
implants. Support by Louisiana Board of Regent grant LEQSF- 2009, 255, 3989–3993.
2009RD is acknowledged. (17) Sukhorukov, G.; Donath, E.; Davis, S.; Lichtenfeld, H.; Caruso, F.;
Popov, V.; Mohwald, H. Stepwise Polyelectrolyte Assembly on
References and Notes Particle Surface: A Novel Approach to Colloid Design. Polym. AdV.
Technol. 1998, 9, 759–767.
(1) Joussein, E.; Petit, S.; Churchman, J.; Theng, B.; Righi, D.; Delvaux, (18) Leporatti, S.; Voigt, A.; Mitlohner, R.; Sukhorukov, G.; Donath, E.;
B. Halloysite Clay Minerals: A Review. Clay Minerals 2005, 40, 383– Mohwald, H. Scanning Force Microscopy Investigation of Polyelec-
426. trolyte Nano- and Microcapsule Wall Texture. Langmuir 2000, 16,
(2) Tari, G.; Bobos, I.; Gomes, C.; Ferreira, J. Modiﬁcation of Surface 8850–8857.
Charge Properties During Kaolinate to Halloysite-7A Transformation. (19) Javier, A. M.; Kreft, O.; Semmling, M.; Kempter, S.; Skirtach, A. G.;
J. Colloid Interface Sci. 1999, 210, 360–369. Bruns, O. T.; del Pino, P.; Bedard, M. F.; Radler, J.; Kas, J.; Plank,
(3) Price, R.; Gaber, B.; Lvov, Y. Release Characteristics of Tetracycline, C.; Sukhorukov, G. B.; Parak, W. J. Uptake of Colloidal Polyelec-
Khellin and NAD from Halloysite: A Cylindrical Mineral for Delivery trolyte-Coated Particles. AdV. Mater. 2008, 20, 4281–4290.
of Biologically Active Agents. J. Microencapsulation 2001, 18, 713– (20) Horcas, I.; Fernandez, R.; Gomez-Rodriguez, J.; Colchero, J.; Gomez-
723. Herrero, J.; Baro, A. M. WSxM: A Software for Scanning Probe
(4) Shchukin, D.; Price, R.; Sukhorukov, G.; Lvov, Y. Biomimetic Microscopy and a Tool for Nanotechnology. ReV. Sci. Instrum. 2007,
Synthesis of Vaterite in the Interior of Clay Nanotubules. Small 2005, 78, 13705.
(21) Treacy, M.; Ebbesen, T.; Gibson, J. Exceptionally High Young’s
(5) Kelly, H.; Deasy, P.; Ziaka, E.; Claffey, N. Formulation and
Modulus Observed for Individual Carbon Nanotubes. Nature 1996,
Preliminary in Vivo Dog Studies of a Novel Drug Delivery System
for the Treatment of Periodontitis. Int. J. Pharm. 2004, 274, 167–
183. (22) Mossman, B.; Churg, A. Mechanisms in the Pathogenesis of Asbestosis
(6) Veerabadran, N.; Price, R.; Lvov, Y. Clay Nanotubules for Drug and Silicosis. Am. J. Respir. Crit. Care Med. 1998, 157, 1666–1680.
Encapsulation and Sustained Release. NANO 2007, 2, 215–222. (23) Hart, G.; Hesterberg, T. In Vitro Toxicity of Respirable-Size Particles
(7) Lvov, Y.; Shchukin, D.; Mohwald, H.; Price, R. Clay Nanotubes for of Diatomaceous Earth and Crystalline Silica Compared with Asbestos
Controlled Release of Protective Agents. ACS Nano 2008, 2, 814– and Titanium Dioxide. J. Occup. EnViron. Med. 1998, 40, 29–42.
820. (24) Wiessner, J.; Mandel, N.; Sohnle, P.; Mandel, G. Effect of Particle
(8) Abdullayev, E.; Price, R.; Shchukin, D.; Lvov, Y. Halloysite Tubes Size on Quartz-induced Hemolysis and on Lung Inﬂammation and
as Nanocontainers for Anticorrosion Coating with Benzotriazole. ACS Fibrosis. Exp. Lung. Res. 1989, 15, 801–812.
Appl. Mater. Interfaces 2009, 2, 1437–1443. (25) Porter, A.; Gass, M.; Muller, K.; Skepper, J.; Midgley, P.; Welland,
(9) Veerabadran, N.; Mongayt, D.; Torchilin, V.; Price, R.; Lvov, Y. M. Direct Imaging of Single-Walled Carbon Nanotubes in Cells. Nat.
Organized Shells on Clay Nanotubes for Controlled Release of Mater. 2007, 2, 713–718.
Macromolecules. Macromol. Rapid Commun. 2009, 30, 94–9. (26) Nel, A.; Xia, T.; Madler, L.; Li, N. Toxic Potential of Materials at
(10) Kommireddy, D.; Ichinose, I.; Lvov, Y.; Mills, D. Nanoparticle the Nanolevel. Science 2006, 311, 622–628.
Multilayer: Surface Modiﬁcation for Cell Attachment and Growth. (27) Yang, Y.; He, Q.; Duan, L.; Li, J. B. Assembled Alginate/Chitosan
J. Biomed. Nanotechnol. 2005, 1, 286–290. Nanotubes for Biological Application. Biomaterials 2007, 18,
(11) Lvov, Y.; Ariga, K.; Ichinose, I.; Kunitake, T. Formation of Ultrathin 3083–3090.
Multilayer and Hydrated Gel from Montmorillonite and Linear
Polycations. Langmuir 1996, 12, 3038–3044. BM9014446